# Modeling the strain-rate dependence of fatigue life of hot-pressed silicon nitride

## Modeling the strain-rate dependence of fatigue life of hot-pressed silicon nitride

**Modeling the strain-rate dependence of fatigue life of hot- pressed silicon nitride Vinod Sharma, S. Nemat-Nasser *, Kenneth S. Vecchio Center of Excellence for Advanced Materials, Department of AMES, 9500 Gilman Drive, University of California, San Diego, La Jolla, CA 92093-0416, USA Received 22 March 1997; revised version received 5 March 1998 Abstract This paper presents the results of a micromechanical model used to explain the strain-rate dependence of the com- pression fatigue lives of amorphous and crystalline grain boundary phase; denoted by ABP and CBP silicon nitrides, respectively. **

When the strain-rate is changed from 400 to 0.01/s, the fatigue lives of both materials, evaluated at a peak stress of 3.2 GPa, increased by more than two orders of magnitude (Sharma et al. (1996a,b)). The model is based on the dynamic and quasi-static microstructural damage mechanisms observed in both materials. The microstructure of ABP and CBP silicon nitrides is modeled as a simple composite in which silicon nitride grains are embedded in a continuous network of the grain boundary phase. Since the subsurface fatigue cracks in both materials nucleate mainly from the contact region between silicon nitride grains, contact stresses between adjacent silicon nitride grains are obtained, and the frequency dependence of the fatigue lives of ABP and CBP silicon nitrides is explained on the basis of the strain-rate sensitivity of the grain boundary phase.

Ó 1998 Elsevier Science Ltd. All rights reserved. 1. Introduction In recent work by the authors (Sharma et al. (1996a,b)), the results of an experimental investi- gation of the eects of the grain boundary phase on the dynamic and quasi-static compression fa- tigue life of hot-pressed silicon nitrides are present- ed. The compression fatigue lives of amorphous grain boundary phase (ABP) and crystalline grain boundary phase (CBP) silicon nitrides are evaluat- ed at strain-rates of 0.01, 0.1 and 400/s. Table 1 summarizes the results of the experiments. ABP silicon nitride was ¯uxed with 6 wt% Y2O3 and 3 wt% Al2O3, whereas CBP silicon nitride was ¯uxed with 8 wt% Y2O3 and 1 wt% Al2O3.

At a strain- rate of 400/s, the fatigue life of ABP silicon nitride (104 cycles) is observed to be superior to the fa- tigue life of CBP silicon nitride (44 cycles). When the strain-rate is decreased from 400 to 0.01/s, the fatigue lives of both materials increases by more than two orders of magnitude and the dier- ence in the fatigue life of ABP silicon nitride (14,000 cycles) and CBP silicon nitride (12,000 cy- cles) was found to be relatively less signi®cant. The observed signi®cant dierences in the fatigue lives between 400 and 0.01/s strain-rates was accredited to the dierences in the energy loss, which is given by the enclosed area within the axial stress±strain curve, in a typical compression fatigue cycle.

The energy loss per cycle, in samples from both materi- als, at a strain-rate of 0.01/s was observed to be Mechanics of Materials 29 (1998) 253±273 * Corresponding author. E-mail: ceam@ames.ucsd.edu. 0167-6636/98/$ ± see front matter Ó 1998 Elsevier Science Ltd. All rights reserved. PII: S 0 1 6 7 - 6 6 3 6 ( 9 8 ) 0 0 0 2 4 - 6

insigni®cant compared to the energy loss in a typ- ical fatigue cycle at 400/s. For ABP and CBP silicon nitrides, the micro- cracks and dislocations were observed to nucleate mainly from the contact region between two sili- con nitride grains. The grains of silicon nitride are generally separated by a grain boundary phase which can be as thin as 1±8 nm (Ahn and Thomas, 1983). For the purpose of numerical analysis, the microstructure of ABP and CBP silicon nitrides is modeled as a composite in which silicon nitride grains are surrounded by a thin boundary phase layer.

When a ceramic is subjected to compression loading, local shear stresses may act on the face of pre-existing ¯aws.

**The shear stress acting on the ¯aws causes the cracks to grow along the ap- plied compression direction under a local tensile ®eld (Nemat-Nasser and Horii, 1982; Horii and Nemat-Nasser, 1986; Ashby and Hallam, 1986). To ®nd the critical sites where fatigue cracks are likely to nucleate, the maximum in-plane shear stress, in the vicinity of contact region, is found by varying the contact radius and the thickness of the intergranular layer.**

The eect of high pressure on amorphous silica was studied by Bridgeman and Simon (1953). They observed that amorphous silica undergoes plastic deformation at pressures of the order of 1 to 10 GPa. Since silica is present in the grain boundary phases, and very high stresses are generated at the contact regions, the grain boundary phases are assumed to have strain-rate sensitive plasticity. The strain-rate dependence of fatigue life is numer- ically modeled based on the strain-rate sensitivity of the grain boundary phases, and the manner by which the forces are transmitted over the contact area between adjacent grains.

In other words, the change in the maximum in-plane shear stress is ex- amined by changing the yield strength of the grain boundary phases to mimic the behavior of a strain- rate sensitive material.

In order to ®nd the elastic constants of amor- phous and crystalline grain boundary phases, an attempt was made to produce these materials from appropriate oxide powders. However, the attempt was not very successful due to the lack of proper facilities. Thus, the average elastic properties of the amorphous grain boundary phase, silicon nit- ride grains and the crystalline grain boundary phase are estimated theoretically. These properties are then used to ®nd the contact stresses as a func- tion of the contact radius and the thickness of the grain boundary phase.

2. Estimation of elastic properties of silicon nitride grains and amorphous and crystalline grain boun- dary phase To evaluate the properties of grain boundary phases, it is important to know their composition.

The composition of each grain boundary phase de- pends upon the relative amounts of sintering aids, as well as upon the impurity content, concentra- tion of silica present on silicon nitride particles, and other factors. Normally, the concentration of oxygen in submicron silicon nitride particles varies from 1±3 wt%. If oxygen were to be present only in the form of silica, then the concentration of silica in silicon nitride particles varies from about 2±6 wt%. In estimating the elastic constants, the concentration of silica in silicon nitride powder is taken to be slightly under 3.5 wt%, which corre- sponds to 3 wt% silica in ABP and CBP silicon nit- rides.

Thus, the composition of the ABP silicon nitride is taken to be: 88 wt% Si3N4, 3 wt% SiO2, 6 wt% Y2O3, and 3 wt% Al2O3, whereas the com- position of the CBP silicon nitride is taken to be: 88 wt% Si3N4, 3 wt% SiO2, 8 wt% Y2O3, and 1 wt% Al2O3. In reality, some of silicon nitride is also present in the grain boundary phase, which is neglected here in the estimation of the properties of intergranular phases and silicon nitride grains. Small additions of silicon nitride to the intergran- Table 1 Variation in compression fatigue lives of ABP and CBP silicon nitrides as a function of strain rate.

**Strain rate ABP silicon nitride CBP silicon nitride 400/sec 104 cycles 44 cycles 400/sec 91 cycles 33 cycles 0.1/sec 9500 cycles 3500 cycles 0.01/sec 14030 cycles 11965 cycles 0.01/sec 12150 cycles 10210 cycles 254 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273**

ular phase increase the hardness and modulus of the grain boundary phase. Thus, the estimated moduli of the crystalline and amorphous grain boundary phase are expected to be lower than the actual moduli. 2.1. Estimate of the elastic properties of amorphous grain boundary phase The elastic properties of certain oxide glasses were calculated from their chemical composition by Mackishima and Mackenzie (1973, 1975).

Their calculation was based on the consideration of the packing density and the dissociation energy of the oxide constituents per unit volume. Accord- ing to them, the Young modulus of an oxide glass is given by E 83:6Vt X n i1 GiXi; 1 where Gi is the dissociation energy per unit volume of component i, Xi is the mole fraction of the ith component, and Vt is the packing density. In Eq. (1), if G is measured in kcal/cm3 then the Young modulus has the units of kbar The packing density is given by Vt q M X n i1 ViXi; 2 where M is the eective molecular weight, q is the density of the glass, and Vi is the packing factor for component i.

Table 2 lists the values of the dis- sociation energy per unit volume and the packing factor for SiO2, Y2O3, and Al2O3.

For 50 wt% Y2O3 + 25 wt% SiO2 + 25 wt% Al2O3 (amorphous grain boundary phase), the ef- fective molecular weight 113.28, density 3.55 gm/cm3 , and the mole fraction of yttria, alumina, and silica are 25.1%, 27.8% and 47.1%, respective- ly. Substituting these values into Eqs. (1) and (2), and using the constants from Table 2, we ®nd the Young's modulus of the glassy phase to be equal to 101.2 GPa. According to Mackishima and Mackenzie (1975), the shear modulus (l) of a glass is given by l 300:96V 2 t 10:8Vt ÿ 1 X n i1 GiXi: 3 Substituting the values of the packing factor, the dissociation energy per unit volume, and the mole fraction of each component (obtained from the calculation of Young's modulus) in Eq.

(3), we obtain the shear modulus of glass as 40 GPa. Once the Young and shear moduli of the amor- phous grain boundary phase are known, other elastic properties can be estimated, assuming isot- ropy. Table 3 lists these estimated properties of the amorphous grain boundary phase.

2.2. Estimate of the elastic properties of silicon nitride grains The concepts of micromechanics can be used to estimate the average elastic constants for the sili- con nitride grains. Here, we shall use the so-called self-consistent method (Kroner, 1958; Budiansky, 1965; Hill, 1965). Assume that the glassy phase is present in the form of spherical inclusions in a ma- trix of silicon nitride grains. Alternatively, we could assume a more realistic situation in which silicon nitride grains are present in the form of Table 2 Dissociation energy per unit volume and packing factor of se- lected oxides (from Mackishima and Mackenzie (1973)) Silica Yttria Alumina Gi(kcal/cm3 ) 15.4 17.7 32 Vi 14 24.8 21.4 Table 3 Measured mechanical properties of ABP and CBP silicon-nitrides CBP silicon-nitride (8% Y2O3,1% Al2O3) ABP silicon-nitride (6% Y2O3,3% Al2O3) Young's modulus 319 GPa 304 GPa Shear modulus 126.2 GPa 120.7 GPa Poisson's ratio 0.264 0.259 Density 3248 kg/m3 3233 kg/m3 V.

Sharma et al. / Mechanics of Materials 29 (1998) 253±273 255

spherical inclusions in a matrix of the glassy phase. In the self-consistent method, the roles of the two phases are interchangeable and the elastic con- stants, estimated by self-consistent method, are not aected by this choice. If the matrix and inclu- sions are assumed to be linearly elastic and isotro- pic, then the elastic constants of silicon nitride grains can be estimated either by a dilute distribu- tion scheme in which the interaction between in- clusions is neglected, or by the self-consistent scheme which accounts to some extent for the in- teraction between grains. Since the volume frac- tion of the glassy phase is greater than 10%, the self-consistent scheme is used to estimate the aver- age elastic constants for silicon nitride grains.

Ac- cording to this scheme, the elastic constants of the composite material (grains and grain boundary phase) are related to the elastic constants of the in- clusions and the matrix through the following rela- tions (Nemat-Nasser and Hori, 1993): K K 1 ÿ f K K ÿ KI K K ÿ KI K K ÿ KI ÿ s1 x1a ÿ1 ; 4 l l 1 ÿ f l l ÿ lI l l ÿ lI l l ÿ lI ÿ s2 x1a ÿ1 ; 5 where f is the volume fraction of inclusions (glassy phase), and K; l; K; l; KI , and lI are the bulk and shear moduli of the matrix, composite, and in- clusions, respectively. s1 and s2 are the components of Eshelby's tensor for spherical inclusions, given by, s1 1 m 3 1 ÿ m ; 6 s2 2 4 ÿ 5m 15 1 ÿ m ; 7 where m is Poisson's ratio of the composite (ABP silicon nitride).

The elastic constants of ABP and CBP silicon nitrides were calculated by measuring the pulse echo sound speed in the longitudinal and shear modes. Table 3 (Sharma et al., 1994) lists the mea- sured elastic constants of ABP and CBP silicon nitrides. By knowing the elastic constants of ABP silicon nitride (composite) and glassy phase (inclusion), Eqs. (4) and (5) can be solved for bulk and shear moduli of silicon nitride grains. The es- timated values of the aggregate properties of sili- con nitride grains are listed in Table 4. 2.3. Estimate of the elastic constants of crystalline grain boundary phase Since the properties of CBP silicon nitride (composite) and silicon nitride grains (matrix) are known, Eqs.

(4) and (5) can be used to estimate the properties of the crystalline grain boundary phase (inclusion). The elastic constants of the crys- talline grain boundary phase are listed in Table 4. It can be observed from Tables 3 and 4 that while most of the properties of ABP and CBP sil- icon nitrides fall between the properties of silicon nitride grains and amorphous/crystalline grain boundary phase, the Poisson ratio of ABP silicon nitride is lower than the Poisson ratio of silicon nitride grains and the glassy phase. This is due to the self-consistent model used to determine the properties of silicon nitride grains from the proper- ties of ABP silicon nitride and the glassy phase.

This model ensures that the modulus of the com- posite falls between the modulus of the matrix and the inclusion. Since Poisson's ratio is a dimen- sionless number, it is not constrained by the prop- erties of the inclusions and the matrix under the self-consistent scheme.

Table 4 Estimated elastic properties of amorphous boundary phase, silicon-nitride grains, and crystalline boundary phase ABP Silicon-nitride CBP Young's modulus 101.2 GPa 345.6 GPa 162.6 GPa Shear modulus 40 GPa 137 GPa 62.8 GPa Poisson's ratio 0.264 0.261 0.295 Bulk modulus 71.4 GPa 241 GPa 132 GPa 256 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

3. Modeling the frequency dependence of fatigue lives of ABP and CBP silicon nitrides In this section, the frequency dependence of fa- tigue lives of ABP and CBP silicon nitrides is mod- eled based on the strain-rate sensitivity of the amorphous and crystalline grain boundary phases.

Since fatigue cracks in ABP and CBP silicon nit- rides initiate from contact regions between two grains, the contact stresses between adjacent sili- con nitride grains, with a thin intergranular layer in between, are calculated numerically. The lattice image of three grains of silicon nit- ride and the grain boundary phase for ABP and CBP silicon nitrides is shown in Fig. 1(a) and (b), respectively (Sharma, 1994; Sharma et al., 1998). A thin amorphous layer is observed be- tween crystalline grain boundary phase and silicon Fig. 1. TEM lattice image of silicon nitride showing (a) amorphous nature of grain boundary phase and (b) partial crystalline nature of grain boundary phase.

V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 257

nitride grains in CBP material in Fig. 1(b), likely due to partial crystallization of crystalline grain boundary phase. The microstructure of CBP sili- con nitride, at a somewhat lower magni®cation, is shown in Fig. 2 (Sharma et al., 1994). Similar microstructure was observed for ABP silicon nit- ride. The microstructure of ABP and CBP silicon nitrides is rather complicated, consisting of several grain sizes and grain morphologies, which makes it dicult to determine the exact state of stress with- in the material.

This task is further complicated by a wide range of thickness of the intergranular lay- er, the possible presence of a thin amorphous layer between crystalline grain boundary phase and sili- con nitride grains in CBP material, the anisotropy of silicon nitride grains and the intergranular lay- er, the presence of dislocations, microcracks, and other factors. For the purpose of obtaining a rough estimate of the contact stress between two impinging grains, the actual microstructure is modeled as a simple two-dimensional periodic mi- crostructure consisting of circular and hexagonal grains with a thin intergranular layer between grains.

Due to the inability to measure the me- chanical properties of the thin amorphous layer present between silicon nitride grains and the crys- tallized grain boundary phase in the CBP material, the grain boundary phase for the CBP material is assumed to be completely crystalline in the present model.

The idealized microstructure of the material is shown in Fig. 3. The periodically distributed unit cell is made up of two hexagonal and two circular grains (shown by dashed lines in Fig. 1). The eect of the contact radius and the thickness of the inter- granular phase on the contact stresses was evaluat- ed by generating dierent repetitive cells. Contact stresses were evaluated for six dierent contact ra- dii (5, 10, 20, 50, 100, 250 nm) and for each contact radius, two dierent thickness (1, 5 nm) were cho- sen. The lateral dimension of the repetitive cell was kept constant (510 nm) and the axial dimension was varied depending upon the contact radius Fig.

2. TEM micrograph showing the microstructure of CBP silicon nitride.

Fig. 3. Idealized periodic microstructure of ABP and CBP sili- con nitrides; this microstructure is used for estimating the con- tact stresses as functions of the contact radius and the thickness of the intergranular phase. 258 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

and thickness of the intergranular phase between hexagonal grains. The distance between parallel sides of the hexagonal grains was kept constant at 500 nm. The area fraction of the grain boundary phase was set at about 11%, by varying the diam- eter of the circular grains.

Dierent meshes for ®nite element analysis were generated by MAZE (Hallquist, 1983) which is an input generator for the actual ®nite element code. Fig. 4 shows a typical repetitive cell. There are about 5500 elements in each mesh; the actual num- ber increases as the thickness of the intergranular layer is increased. When the contact radius of the hexagonal grains is equal to 250 nm, the hexagonal grains collapse into circular grains. Fig. 5 shows a repetitive cell for a contact radius of 250 nm. The average elastic constants of the repetitive cell are the same as those of ABP/CBP silicon nit- ride.

However, the elastic constants vary widely within the plane of the repetitive cell. As a result, Fig. 4. Schematic diagram of a typical mesh used to analyze contact stresses between two grains with a thin intergranular layer between them.

V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 259

the pressure boundary condition does not give rise to uniform displacements. To achieve uniform boundary displacements (a more realistic situa- tion), the displacement boundary conditions were speci®ed on all four sides of the repetitive cell. The axial displacements on the boundaries were speci®ed according to dlaxial rzzlaxial/E, where laxial is the axial length of the repetitive cell, rzz is the peak applied stress (3.2 GPa) used in the fa- tigue experiments (Sharma et al., 1996a,b), and E is the Young's modulus of the ABP/CBP silicon nitride.

The lateral displacement was speci®ed ac- cording to the relation dllateral mrzzllateral/E, where m is the Poisson ratio of ABP/CBP silicon nitride and llateral is the lateral dimension of the repetitive cell (510 nm).

The contact problem was analyzed using NIKE2D (Hallquist, 1979, 1986). NIKE2D is an implicit ®nite element code for analyzing the ®nite deformation, static, and dynamic response of two- dimensional axisymmetric, plane strain and plane stress solids. All calculations were performed for the plane strain geometry. We point out again that this gives only a rough estimate of the stress state, Fig. 5. Typical ®nite-element mesh for a contact radius of 250 nm; each unit cell involves approximately 5500 elements. 260 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273

as the actual situation is neither two-dimensional nor periodic.

The elastic constants for crystalline and amor- phous grain boundary phases and silicon nitride grains, estimated in the previous section, were used as an input to NIKE2D. The output of NIKE2D was used in ORION (Hallquist and Levatin, 1985), which is a post-processor for NIKE2D, to ®nd the contact stresses. Once the stress tensor within each element is known, the maximum in- plane shear stress {(syz)max} was found from the following relation: syzmax rzz ÿ ryy 2 n o2 s2 yz r ; 8 where rzz is the axial stress, ryy is the lateral stress and syz is the shear stress within an element.

4. Upper and lower bounds on the elastic moduli based on the periodic microstructure Bounds on the overall elastic moduli of a peri- odic microstructure can be found by homogenizing the microstructure and minimizing the strain ener- gy and complementary strain energy of the ho- mogenized microstructure (Nemat-Nasser et al., 1982; Nemat-Nasser and Hori, 1993). The micro- structure can be homogenized by choosing an arbi- trary reference material and by prescribing suitable eigenstrain (eigenstress) ®elds to accommodate the material mismatch. If the matrix is stier than the inclusion, then the upper bound is obtained by choosing the reference material to be the same as the matrix material, and the lower bound is ob- tained when the reference material is chosen as the inclusion material.

For a two-phase composite material, the upper and lower bounds on the elas- tic moduli are given by (Nemat-Nasser and Hori, 1993; Nemat-Nasser et al., 1993), C CM fX CX ÿ CM ÿ1 fXCXX CM h iÿ1 ; 9 C ÿ CX 1 ÿ fX CM ÿ CX ÿ1 f 2 X 1 ÿ fX CXX CX ÿ1 ; 10 where fX is the volume fraction of inclusions, CM and CX are the elasticity tensor for matrix and in- clusions, respectively, and CXX is the function of the reference elasticity tensor and the geometry of the inclusion.

Universal upper and lower bounds can be ob- tained based on only the volume fraction of the in- clusions, without considering the geometry of the inclusion in the calculation of CXX . The CXX matrix in this case is given by the following relations (Ne- mat-Nasser and Hori, 1993): fXCXX iijj 1 ÿ fX 1 ÿ 2m 2l 1 ÿ m ; 11a fXCXX ijij 1 ÿ fX 3 ÿ 4m 2l 1 ÿ m ; 11b where l is the shear modulus and m is Poisson's ra- tio of the reference material. For an isotropic material, the two-dimensional stiness matrix for plane strain geometry is given by E 1 ÿ m 1 m 1 ÿ 2m Em 1 m 1 ÿ 2m Em 1 m 1 ÿ 2m E 1 ÿ m 1 m 1 ÿ 2m 0 0 E 1 m ; 12 where E is the Young modulus of the reference material.

The elasticity tensor for the matrix and the inclusion can be obtained by substituting E and n into the above equation. Substituting CM , CX , and Eq. (12) into Eqs. (9) and (10), the univer- sal upper and lower bounds are found as, C U 540:12 282:68 0:0000 282:68 540:12 0:0000 0:0000 0:0000 334:80 ; 13a C ÿ U 374:71 117:28 0:0000 117:28 374:71 0:0000 0:0000 0:0000 223:84 ; 13b If the geometry of the inclusion is also account- ed for in the determination of the bounds, then CXX is given by the following relation: CXX X 1 n gX ÿngX n^ C n; C: 14 V. Sharma et al. / Mechanics of Materials 29 (1998) 253±273 261